Grade 1.4034 - 420 Stainless Steel
1.4034 is a martensitic grade of 420 stainless stainless. It is magnetic and hardenable with rust resistant properties. 1.4034 stainless is characterised by having a 0.43-0.50 carbon, and 12.5-14.5% chromium content. This mix of analysis gives our 1.4034 stainless sheet and sections an outstanding corrosion resistance and exceptional wear properties after heat treatment. Superior to 410 and 416 type stainlesses for most applications. 1.4034 stainless steel has good ductility in the annealed condition, but is capable of achieving 57HRC after treatment. Optimal corrosion resistance is realised when 1.4034 is surface ground and polished after hardening.
|1.4034 - 420 Stainless Steel Chemical Analysis wt %|
|0.43-0.50||≤ 1.00||≤ 1.00||≤ 0.04||≤ 0.015||12.5-14.5||≤ 1.00|
Applications for 1.4034
Dental and surgical instruments cutlery pump shafts gear pinions, cams, various hand tools, straight edges, parts for firearms and scissors
Not recommended for high pressure vessels.
Soft Annealing 1.4034
Heat to 730-780°C. Cool slowly in air.
Structure is ferrite with spherical carbides.
Good machining characteristics due to the addition of Sulphur.
High speeds and feeds producing short brittle chips
|1.4034 - 420 Stainless Mechanical Properties at ambient temperature|
Condition annealed. Quenched and tempered 850°C
0.2% Proof Stress: 650 Nmm²
Tensile Strength: 850 - 1000 Nmm²
Hardness HB Max 230
Hot forming temperature 800-1100°C. Slow cool
Harden from a temperature 980-1030°C
Follow by oil or air quenching.
Hardness after quenching 52-58 HRC
Tempering temperature 100-200°C
Heat Treatment Advise of 1.4034
Treatment temperatures, including the rate of heating, cooling and soaking times will vary due to factors such as the shape and size of each 420 stainless steel component. other considerations during the heat treatment process include the type of furnace, quenching medium and work piece transfer facilities. Please consult your heat treatment provider for full guidance for the heat treatment of 1.4034
Corrosion resistance 1.4034
Hardened condition realises resistance to atmosphere, fresh, dilute acids and alkalise, fresh water and fruit and vegetable juices
|1.4034 - 420 Stainless Steel Physical properties|
Average values at ambient temperature
Modulus of elasticity. (10³ x N/mm2) : 220
Density. (g/cm³): 7.74
Thermal conductivity. (W/m.K): 30.0
Electric resistivity. (Ohm mm²/m): 0.65
Specific heat capacity. (J/g.K): 0.46
Welding of 1.4034
Not commonly welded due to its air hardening characteristics. Welding may possibly be performed after preheating to 150-205°C with the post welding tempering at temperature for 2 hours. Recommendation of specialist advice to be sought
Cold working of 1.4034
Material will withstand only minor cold work. Radical forming operations will result in cracking
The information and data presented herein are typical or average values and are not a guarantee of maximum or minimum values. Applications specifically suggested for material described herein are made solely for the purpose of illustrations to enable the reader to make their own evaluations. They are not intended to either express or imply the suitability for these or any other purposes